- Nano Express
- Open Access
Wettability Modification of Nanomaterials by Low-Energy Electron Flux
© to the authors 2009
- Received: 9 March 2009
- Accepted: 15 June 2009
- Published: 2 July 2009
Controllable modification of surface free energy and related properties (wettability, hygroscopicity, agglomeration, etc.) of powders allows both understanding of fine physical mechanism acting on nanoparticle surfaces and improvement of their key characteristics in a number of nanotechnology applications. In this work, we report on the method we developed for electron-induced surface energy and modification of basic, related properties of powders of quite different physical origins such as diamond and ZnO. The applied technique has afforded gradual tuning of the surface free energy, resulting in a wide range of wettability modulation. In ZnO nanomaterial, the wettability has been strongly modified, while for the diamond particles identical electron treatment leads to a weak variation of the same property. Detailed investigation into electron-modified wettability properties has been performed by the use of capillary rise method using a few probing liquids. Basic thermodynamic approaches have been applied to calculations of components of solid–liquid interaction energy. We show that defect-free, low-energy electron treatment technique strongly varies elementary interface interactions and may be used for the development of new technology in the field of nanomaterials.
- Low-energy electron irradiation
- Thermodynamic properties
Finely divided submicron and nanoscale solid materials demonstrate anomalous properties at both nano- and microscales due to their huge surface energy and high specific surface area. They are considered today as building blocks in many nanotechnological applications related to electronics, optics and biomedicine . Many diverse fundamental surface-related physical properties of nanomaterials such as wettability, dispersion, hygroscopicity and agglomeration define key nanotechnological processes .
The common physical property of nanomaterials is to create macroscopic aggregates. For example, cohesion followed by agglomeration easily occurs among ZnO nanoparticles due to their huge specific surface area, high intrinsic surface energy  as well as pyroelectric electrostatic interaction . Agglomeration leads to a nonuniform density distribution of the nanomaterials. However, the most obvious effect of agglomeration is losing of individual physical properties of nanoparticles, especially physical properties provided by quantum-size effects. Self-assembled nanomaterials strongly demonstrate different basic features and figures of merit compared to individual nanoparticles of the same composition. Thus, nanopowder surface modification, preventing or strengthening cohesion and agglomeration of nanoparticles, is a critical issue in nanotechnology .
Fundamental studies [6, 7] have been recently undertaken to understand interparticle forces leading to assembly or nonassembly of nanoparticles. Numerous research works on fine nanomaterial surface treatment technology have been directed to change their affinity to agglomeration. It has been shown that aggregation can be prevented by protecting nanoparticles using polymer or surfactant monolayers. Another way is electrical charging electrostatic stabilization, which is used in aqueous solutions where the particles are surrounded by a hydration layer, preventing their coalescence . Various “encapsulation” technologies have been applied using different chemical materials, to decrease or to increase the nanoparticles surface energy and their intrinsic affinity to cohesion and agglomeration [8–10]. It has become clear that wettability is a critical factor in the creation of nanoparticle clusters . The surface modification of nanomaterials, providing transition from hydrophobic (low surface energy) to hydrophilic (high surface energy) state or vice versa, has many potential applications in many fields of modern nanotechnology such as prevention of aggregation of the particles , modification of chemical stability, variation of their tribological properties and improving biocompatibility of nanomaterials .
Recently, a new approach has been developed by us to modify materials surface free energy and many related properties  such as wettability , bonding , etching  and biocompatibility [17, 18]. This technique is based on combination of ultraviolet (UV) illumination and low-energy electron irradiation. UV treatment is a well-known technique for the surface modification leading to hydrophilicity enhancement of materials . The method of low-energy electron irradiation has been developed in our laboratory for surface energy modification of solid-state materials of different origins [13, 20]. The key principle of the method developed is that the chosen electron energy is much less than the energy threshold of defects creation in irradiated materials. The electron current, incident electron charge and electron energy are coadapted to the electronic structures of the materials when the injected primary electrons and generated secondary electron/hole charges are trapped near the surface at the depth of a few nanometers . We observed this phenomenon in many solid-state materials, such as amorphous SiO2, S3N4, glass, mica, Al2O3, n- and p-Si, metal oxides (TiO2, Al2O3, ZnO thin films), biomimetic and biomaterials (sea shells, hydroxyapatite and related calcium phosphates). The wettability of ferroelectric LiTaO3 crystal has been varied in a range of contact angles from high hydrophilic (water contact angle θ = 6°) to hydrophobic state with θ = 90°. It has afforded to find optimal conditions for direct bonding of ferroelectric crystals . Two different mechanisms of hydrophobicity enhancement versus incident electron charge have been found, where one is surface electrostatic charging observed for low level of electron incident charge and the other is formation of ultrathin organic film, which was observed for high-electron doses .
In this paper, we apply the method of low-energy electron treatment  to powders of different origins, such as diamond and ZnO. Diamond powder possesses exceptional chemical inertness that arises from high atomic density and strong intrinsic covalent bonding .The agglomeration of diamond powder is observed for nanoparticles with dimensions less than 100 nm. However, the larger the size of nanoparticles the less is the affinity to agglomeration . Another nanomaterial, ZnO, is unique and widely studied. Its low chemical stability and well-defined catalytic and pyroelectric properties allow observing high affinity to cohesion and agglomeration leading to the formation of various self-assembled nanostructures such as nanowires and nanorings . Photosensitivity of ZnO is the physical reason for photoinduced wettability conversion .
The controllable nanoscale modification of surface free energy and related properties described in this work using low-energy electron flux is a new promising concept for nanomaterials and provides a highly potential approach for the development of new nanotechnology. This nanoscale tool has never been used for modification of nanomaterials.
Low-Energy Electron Treatment Technique
In this work, the combination of two different techniques was used for surface energy modification: UV and low-energy electron irradiation. The UV illumination of nanomaterial samples was carried out using nonfiltered, unfocused UV light (185–2,000 nm) generated by a Hg–Xe lamp. The illumination duration was around 5 min, and it always led to hydrophilic state . The electron irradiation was performed using an electron gun (EPG-7, Kimball Physics Inc., USA) in vacuum 10−7 Torr at room temperature, using invariable energy of the incident electrons Ep = 300 eV. The electron irradiation dose was 360 μC/cm2, which provided a high level of electron-induced hydrophobicity. The particles were being shaken during the UV or low-energy electron irradiation in order to irradiate the whole surface of the treated nanomaterial.
Wettability studies on planar solid surfaces are usually conducted by direct contact angle observation. We applied this method to the observation of a macroscopic variation of the nanomaterial wettability. It was roughly estimated by measuring the static contact angles of sessile drops of deionized water (pH 5.5, resistivity >17 MΩ cm). The plastic adjustable volume pipette (Eppendorf Research®pro, Germany) was used.
Macroscopic wettability of nanomaterials was studied using samples fabricated by covering the nanopowder of the chemically cleaned glass substrate (1 cm2). No mechanical pressure was applied. The thickness of the studied nanoparticle layers was around 1 mm. The macroscopic wettability state of the samples and glass substrate was estimated by measuring the static contact angles of sessile water drops placed on a sample surface. The volume of the water drops was kept constant at 2 μL over measurements. The measured wettability contact angle of the glass substrate was 15–20°.
Such a direct approach of the contact angle measurements cannot be used for high accuracy wettability measurements on finely dispersed solid materials such as nanomaterials. The conventional investigation method followed in this case is capillary rise technique , which leads to a large spectrum of analytical information and is extensively applied in the pharmaceutical industry for wettability studies of nanopowders . Such information is important in drug manufacturing (adhesion or nonadhesion of the component on mixing surface) . However, the capillary rise method strongly limits wettability contact angle measurements to contact angles <90° .
where μ is the liquid viscosity, h is the height of liquid penetration into the powder in time t γLV is surface tension of the liquid in equilibrium with the vapor of the liquid, and rc is radius of the capillary as the powder is considered as a bundle of parallel capillaries of constant radius.
The experimental procedure included several steps. A definite amount of nanoparticles were manually packed in a glass tube (0.5 cm inner diameter and 10 cm long). Before packing with the powder, the glass tubes are thoroughly cleaned with distilled water and then dried at 110 °C. The tube was always filled to the same height and with the same weight for a uniform and constant package of nanoparticles. This column is then placed in upright position in a beaker containing the appropriate probing liquid, and the liquid rise is followed as a function of time. The height was measured with a graduated scale by charge-coupled device camera. The capillary radiusrc(Eq. 1) was determined usingn-hexane, which was found to completely wet the studied samples. Once the value ofrcwas obtained, it was then possible to calculate the contact angle for a given liquid on the powdered surface using the Washburn equation (Eq. 1).
The standard set of 97–99% purity probing liquids possessing well-studied physical properties used in this work were as follows:n-hexane, 1-bromonaphthalene, diiodomethane, formamide, ethylene glycol and water. They differ by their viscosity, surface tension, polar and dispersive components, etc. that allow studying the effect of surface modification of nanomaterials using quantitative analyses of wettability data.
Basic Thermodynamic Approaches
The fundamental basis for understanding fine mechanisms of surface modification of nanomaterials is to carry out a detailed investigation into the surface free energy and its components allowing finding elementary interface interactions. Calculation of surface free energy of solid materials is based on measurements of the wettability contact angles of selected polar and apolar liquids deposited on surfaces [30, 31]. The key methods of calculations of critical surface tension, surface free energy and its components applied in this work are those of Zisman , Owens–Wendt  and a relatively new method of van Oss-Chaudhury-Good .
where γLV is the surface tension of the liquid.
Surface tension (γlv) and its dispersive ( ) and polar ( ) components (in mJ/m2) of the used probing liquids 
Studied Powder Materials
Two different sorts of powders of different origins, having different physical properties, particle size and chemical activity, were selected for the wettability studies. The ZnO nanomaterial (EPM-E from Umicore, Belgium) was of 99.4% purity. The surface area was 1–3 m2/g. The average particle size was 200 nm. The diamond particles (Sinai Yehuda, Israel) had an average size of 1 micron.
Environmental scanning electron microscope Quanta 200F (SEM method) was used to characterize ZnO and diamond powders. The samples were prepared by covering the powder on a glass substrate. No any mechanical pressure was applied during the sample preparation.
SEM Characterization of Powders
SEM image of the diamond material (Fig. 1b) demonstrates absolutely different physical state of these particles. Diamond grains are approximately of a similar shape and around 1 μm in size. The image neither shows agglomerates nor any trends of these diamond particles to self-assembling.
Macroscopic Wettability of Modified Powder
Electron irradiation dramatically changed the liquid drop behavior on the ZnO nanomaterial sample surface (Fig. 2b, c). The droplet that brought into direct contact with the electron-treated nanopowder surface demonstrated a strong resistance to be placed on the surface. The Fig. 2b shows the deformed droplet shape that was generated by the pipette, pressing the droplet to the surface. We did not succeed in “pasting” the droplet to the surface. Very high hydrophobicity (Fig. 2c) was observed when the droplet was dropped down on the ZnO surface from a height of about 3–5 mm. Sometimes the landing water droplets showed bouncing effect caused by high repelling surface properties, resulting in detachment of the drops.
These results clearly demonstrate that the water droplets completely spread on untreated ZnO nanomaterial surface, while they exhibit opposite, strongly hydrophobic behavior on the electron-treated sample. It should be marked that diamond powder did not reveal any variation of the macroscopic wettability state for all kinds of samples (as-prepared, UV-treated and low-energy electron-irradiated). The water droplet demonstrated a fast penetration between diamond particles.
Wettability Studies (Capillary Rise Technique) and Thermodynamic Properties of Modified Powders
Contact angle, θ, measured for as-prepared and treated diamond powders, obtained by the capillary rise technique
As-prepared diamond powder
35 ± 3
54 ± 2
76 ± 1
62 ± 2
75 ± 1
38 ± 2
54 ± 2
69 ± 3
52 ± 2
70 ± 1
35 ± 2
70 ± 1
80 ± 2
80 ± 3
84 ± 2
These experimental data show that as-prepared diamond powder demonstrates a water contact angle of 75° and possesses moderate hydrophobicity. Both UV and electron beam irradiation change rather feebly the wettability for all studied probing liquids with deviation of the contact angles in a very limited range, i.e. Δθ ~ 5–15°.
Contact angle, θ, measured for as-prepared and treated ZnO nanomaterial
As-prepared ZnO nanomaterial
9 ± 1
63 ± 1
66 ± 2
52 ± 3
60 ± 4
8 ± 2
14 ± 2
64 ± 1
20 ± 3
3 ± 1
8 ± 1
72 ± 1
70 ± 2
73 ± 3
85 ± 2
The wettability for as-prepared ZnO nanomaterial sample may be defined as slightly hydrophilic with θ ~ 60°. Under UV illumination, water contact angle dropped down to a very small value of about 3°, which is the evidence that UV modification leads ZnO surface to a high hydrophilic state. All tested liquids, except diiodomethane, showed very low contact angle on UV-treated ZnO powder. These data are consistent with the results of the work  where high photocatalitic properties of ZnO making it hydrophilic have been found. Low-energy electron treatment strongly modified the wettability by strengthening its hydrophobic state especially for the probing liquids with large polar components of the surface free energy [ethylene glycol, formamide, water (Table 1)]. For instance, the water contact angle increased from 3° after UV illumination to 85° after electron treatment.
Identical tendency was found for ZnO nanomaterial (Fig. 3b). The data show that the critical surface tension for untreated ZnO powder is approximately 37 versus 27 mJ/m2for diamond particles. The low-energy electron irradiation leads to the decrease in critical surface tension from 37 to 29 mJ/m2. As a result of the UV treatment, it increases significantly to 70 mJ/m2, providing high hydrophobic state of this nanomaterial. Thus, the range of the critical surface tension modification in ZnO is Δ = 41 mJ/m2, which exceeds the same parameter of the diamond particles by 4.5 times where Δ = 9 mJ/m2.
The calculated data (Table 4) illustrate that both surface modification UV treatments and electron beam weakly change the surface free energy and its components of diamond powder. The dispersive component decreases feebly from 24.5 to 24 mJ/m2after UV treatment, the polar component grows from ~8.5 mJ/m2 to ~13 mJ/m2, leading the fraction relation to . Low-energy electron treatment of diamond particles is characterized by weak reduction in the surface energy and its components (mainly the polar component) of the irradiated material.
ZnO demonstrates high affinity to the surface modification. UV illumination leads to increasing surface free energy valueγsvfrom 40.5 to 66 mJ/m2. The found variations are mainly provided by the contribution of the polar component. It strongly grows from ~18.5 mJ/m2 to ~45 mJ/m2, leading the fraction relation to . Such a growth found for the modified diamond powder was much weaker with . These data are consistent with the critical surface tension measurements (Fig. 3). As a result of UV illumination of ZnO nanomaterial surface, high hydrophilic behavior was observed (Fig. 2a). Low-energy electron treatment was characterized by the opposite effect. Decrease in the surface free energy to 34 mJ/m2was found, which occurs due to decrease in the polar component twice from ~18.5 mJ/m2 to ~9 mJ/m2, while the dispersive component increased slightly up to 25 mJ/m2. The fraction relation falls down to 0.35. Combination of these two modification methods varied the surface free energy in a wide range of 34–66 mJ/m2.
Thus, for both studied powders, surface free energy and wettability modification occurred due to variation of the polar components. This conclusion was also confirmed by our calculations using van Oss-Chaudhury-Good approach , which showed dramatic variation of electron-acceptor component related to a polar sort of surface interactions.
The experiments conducted and the implemented estimations allow finding basic features of surface modification of two powders of different origins, diamond and ZnO. UV illumination leads to increasing the surface free energy making the surface hydrophilic, while the electron treatment generates an opposite effect and induces hydrophobicity. The found modifications are highly pronounced for ZnO nanomaterial and look much weaker for diamond particles. Both methods vary the polar component of surface free energy. UV treatment increases this component, but the electron irradiation decreases it.
The observed variation of the polar component is a direct evidence of deep modification of elementary physical interactions with the studied surfaces. Polar interactions include a few basic purely electrostatic interactions that involve the charge of ions and the permanent dipole of polar molecules. Charge–charge, charge–dipole and dipole–dipole interactions (Debye interactions) belong to this category as well as orientation interactions (Keesom interactions). UV treatment of diamond particles, strengthening the polar component, decreases slightly the dispersive component. UV light causes decomposition of organic contaminations on solid surfaces and leads to surface cleaning [38, 39]. It stimulates adsorption of atmospheric water on the diamond surface . Such a modification leads to increasing its hydrophilic state.
Our experimental data show that UV illumination influences much stronger ZnO nanomaterial occurring due to the enhancement of the polar component. ZnO possesses wurtzite hexagonal structure affording spontaneous electrical polarization and consequently piezoelectricity and pyroelectricity. Its UV-induced strong hydrophilicity may be ascribed to two different factors increasing polar forces: electrostatic interaction of a pyroelectric origin and its photosensitivity. High-energy photons supplied by UV source generate electron–hole pairs in ZnO nanomaterial that leads to the formation of surface oxygen vacancies and Zn+ defective sites . The water and oxygen molecules may coordinate on the photogenerated surface defective site, which leads to dissociative adsorption of the water molecules on the surface. The defective sites on ZnO surface are kinetically more favorable for hydroxyl adsorption than for oxygen adsorption , and as a result, the surface hydrophilicity is dramatically improved and the water contact angle on ZnO nanomaterial surface changes from 60° to 3°. It should be noted that the same considered polar forces of various origins provide extremely high affinity of ZnO nanoparticles to self-assembling into ordered nanostructures  due to the enhancement of cohesive interactions followed by agglomeration (Fig. 1a). It should be marked that the UV variation of hydrophilicity is much weaker in diamond particles as well as its affinity to agglomerate where diamond intrinsic inertness is unique and cannot be sufficiently modified.
The observed growth of hydrophobicity in both sorts of powders under low-energy electron irradiation and the observed decreasing of polar component may be explained by electron-induced formation of carbon-rich layer on the surface. This phenomenon has been observed by us in more than 20 solid-state materials of different origins [13, 21]. In the work of Hillier , it has been shown that the carbon contamination deposited under electron beam irradiation is formed by the reaction of the incident electrons with organic molecules on the irradiated surface. The electron-deposited organic CH2-layer [20, 21] possesses major dispersive component and leads to a strong hydrophobicity.
Pronounced effect of electron-induced surface modification was found for macroscopic wettability behavior of ZnO nanomaterials (Fig. 2). High hydrophilic state induced by UV illumination was converted to extremely high hydrophobic state due to low-energy electron irradiation. It should be noted that the wettability effect is very sensitive to surface defects [42, 43], which might be generated by the electron beam. The applied electron irradiation energy in our experiments was Ep = 300 eV. The chosen electron energy is less by 3 orders of magnitude than the threshold energy for atomic displacement in ZnO and generation of point defects in its lattice . So far, unusually high hydrophobicity observed on ZnO nanomaterial was generated due to the modification of elementary interface interaction forces. Obviously, such a strong water repellency induced by electron irradiation is amplified by highly developed surface area of the nanomaterial.
We have conducted studies of surface modification and basic interface interactions in two powders of different origins, diamond and ZnO. The developed surface modification technique based on combination of low-energy electron irradiation and UV illumination has resulted in surface free energy and wettability modification in a wide range of water contact angles. It has been shown that UV illumination turns the ZnO nanomaterial surface to high hydrophilic state, while a low-energy electron irradiation leads to water repellency. Much weaker wettability modification was observed in diamond particles. The found difference is related to inherent different physicochemical natures of ZnO and diamond powders.
Detailed thermodynamic studies using different classical approaches have allowed us to show that UV and electron beam irradiation strongly modify the surface free energy due a deep modulation of its polar component, resulting in variation of elementary surface interactions.
The electron-induced modification of the surface free energy is a completely new concept for nanomaterials, and the present work proposes an effective technological approach for controlling variation of their key surface-related properties such as wettability, cohesion and agglomeration.
This work was supported by the Israel Science Foundation, grant number 960/05.
- D.K. Pritchard (2004), HSL Report EC/04/03. Published on HSE websiteGoogle Scholar
- Lazghab M, Saleh K, Pezron I, Guigon P, Komunjer L: Powder Technol.. 2005, 157: 79. COI number [1:CAS:528:DC%2BD2MXhtVyrsb7E] 10.1016/j.powtec.2005.05.014View ArticleGoogle Scholar
- Nichols G, Byard S, Bloxham MJ, Botterill J, Dawson NJ, Dennis A, Diart V, North NC, Sherwood JD: J. Pharm. Sci.. 2002, 91: 2103. COI number [1:CAS:528:DC%2BD38XntlCqt70%3D] 10.1002/jps.10191View ArticleGoogle Scholar
- Uematsu K, Morohashi H, Morimoto T, Uchida N, Saito K: J. Mater. Sci. Lett.. 1989, 8: 1011. COI number [1:CAS:528:DyaL1MXlsl2nu74%3D] COI number [1:CAS:528:DyaL1MXlsl2nu74%3D] 10.1007/BF01730471View ArticleGoogle Scholar
- Jung SH, Park SH, Lee DH, Kim SD: Polym.Bull.. 2001, 47: 199. COI number [1:CAS:528:DC%2BD3MXovVyrtbo%3D] 10.1007/s002890170012View ArticleGoogle Scholar
- Kudrolli A: Nat. Mater.. 2008, 7: 174. COI number [1:CAS:528:DC%2BD1cXisVSrsrg%3D]; Bibcode number [2008NatMa...7..174K] 10.1038/nmat2131View ArticleGoogle Scholar
- Min Y, Akbulut M, Kristiansen K, Golan Y, Israelachvili J: Nat. Mater.. 2008, 7: 527. COI number [1:CAS:528:DC%2BD1cXnslKqsrc%3D]; Bibcode number [2008NatMa...7..527M] 10.1038/nmat2206View ArticleGoogle Scholar
- Bayer C, Karches M, Matthews A, von Rohr PR: Chem. Eng. Technol.. 1998,21(5):427. COI number [1:CAS:528:DyaK1cXjtlKisrY%3D] 10.1002/(SICI)1521-4125(199805)21:5<427::AID-CEAT427>3.0.CO;2-HView ArticleGoogle Scholar
- Gang W, Yuedong M, Shaofeng Z, Feng L, Zhongqing J, Xingsheng S, Zhaoxing R, Xiangke W: Plasma Sci. Technol.. 2008,10(1):78. 10.1088/1009-0630/10/1/17View ArticleGoogle Scholar
- Vollath D, Szab’o DV: J. Nanopart. Res.. 1999, 1: 235. COI number [1:CAS:528:DC%2BD3cXivFamtQ%3D%3D] 10.1023/A:1010060701507View ArticleGoogle Scholar
- Pukánszky B, Fekete E: Adv. Polym. Sci.. 1999, 139: 1436.Google Scholar
- Chu PK, Chen JY, Wang LP, Huang N: Mater. Sci. Eng: R: Reports.. 2002,36(5–6):143. 10.1016/S0927-796X(02)00004-9View ArticleGoogle Scholar
- G. Rosenman, D. Aronov, Yu. Dekhtyar, Wettability Engineering in Solid State Materials. PCT Patent, WO 2007/049380 A1, 2007Google Scholar
- Aronov D, Molotskii M, Rosenman G: Appl. Phys. Lett.. 2007, 90: 104104. Bibcode number [2007ApPhL..90j4104A] 10.1063/1.2711656View ArticleGoogle Scholar
- Torchinsky I, Rosenman G: Appl. Phys. Lett.. 2008, 92: 052903. Bibcode number [2008ApPhL..92e2903T] 10.1063/1.2841706View ArticleGoogle Scholar
- Sabaev V, Aronov D, Rosenman G: Appl. Phys. Lett.. 2008, 93: 1444104.Google Scholar
- Aronov D, Rosen R, Ron EZ, Rosenman G: Process Biochem.. 2006, 41: 2367. COI number [1:CAS:528:DC%2BD28XhtFertLfE] 10.1016/j.procbio.2006.06.006View ArticleGoogle Scholar
- Aronov D, Rosen R, Ron EZ, Rosenman G: Surf. Coat. Technol.. 2008, 202: 10–2093. 10.1016/j.surfcoat.2007.08.060View ArticleGoogle Scholar
- Quere D: Rep. Prog. Phys.. 2005, 68: 2495. Bibcode number [2005RPPh...68.2495Q] 10.1088/0034-4885/68/11/R01View ArticleGoogle Scholar
- Aronov D, Rosenman G: Surf. Sci.. 2007, 601: 5042. number [1:CAS:528:DC%2BD2sXht1akt7zE]; Bibcode number [2007SurSc.601.5042A] 10.1016/j.susc.2007.09.003View ArticleGoogle Scholar
- Aronov D, Molotskii M, Rosenman G: Phys. Rev. B.. 2007, 76: 035437. Bibcode number [2007PhRvB..76c5437A] 10.1103/PhysRevB.76.035437View ArticleGoogle Scholar
- Larsson K, Björkman H, Hjort K: J. Appl. Phys.. 2001,90(2):15. 10.1063/1.1376671View ArticleGoogle Scholar
- Krueger A: Adv. Mater.. 2008, 20: 2445. COI number [1:CAS:528:DC%2BD1cXotF2gurc%3D]; Bibcode number [2008ipid.book.....K] 10.1002/adma.200701856View ArticleGoogle Scholar
- Wang ZL, Phys J: Condens. Matter.. 2004, 16: R829. COI number [1:CAS:528:DC%2BD2cXmtVyhtLY%3D]; Bibcode number [2004JPCM...16R.829W] 10.1088/0953-8984/16/25/R01View ArticleGoogle Scholar
- Sun R-D, Nakajima A, Fujishima A, Watanabe T, Hashimoto K: J. Phys. Chem. B. 2001, 105: 1984. COI number [1:CAS:528:DC%2BD3MXhtFynsL0%3D] 10.1021/jp002525jView ArticleGoogle Scholar
- Siebold A, Walliser A, Nardin M: J. Colloid. Interface Sci. 1997,186(1):60. COI number [1:CAS:528:DyaK2sXotV2mtQ%3D%3D] 10.1006/jcis.1996.4640View ArticleGoogle Scholar
- Prestidge CA, Tsatouhas G: Int. J. Pharm.. 2000,198(2):201. COI number [1:CAS:528:DC%2BD3cXitlelurc%3D] 10.1016/S0378-5173(00)00341-0View ArticleGoogle Scholar
- Tüskea Zs, Regdon G, Erősa I, Srčičb S, Pintye-Hódi K: Powder Technol.. 2005,155(2):169.Google Scholar
- Washburn EW: Phys. Rev.. 1921, 17: 273. Bibcode number [1921PhRv...17..273W] 10.1103/PhysRev.17.273View ArticleGoogle Scholar
- Luner P, Oh E: Colloids surf A. Physicochem Eng Asp.. 2001, 181: 31. COI number [1:CAS:528:DC%2BD3MXhs1aqt7Y%3D] 10.1016/S0927-7757(00)00805-0View ArticleGoogle Scholar
- Siboni S, Della Volpe C, Maniglio D, Brugnara M: J. Colloid. Interface Sci.. 2004, 271: 454. COI number [1:CAS:528:DC%2BD2cXht1anu74%3D] 10.1016/j.jcis.2003.09.050View ArticleGoogle Scholar
- Fox HW, Zisman AW: J. Colloid. Sci.. 1950, 6: 514. 10.1016/0095-8522(50)90044-4View ArticleGoogle Scholar
- Owens DK, Wendt RC: J. Appl. Polym. Sci.. 1969, 13: 1741. COI number [1:CAS:528:DyaF1MXltFegtLc%3D] 10.1002/app.1969.070130815View ArticleGoogle Scholar
- Van Oss CJ, Good RJ, Chaudhury MK: Langmuir.. 1988, 4: 884. 10.1021/la00082a018View ArticleGoogle Scholar
- Jańczuk W, Wójcik W, Zdziennicka A: J. Colloid. Interface Sci.. 1993, 157: 384. 10.1006/jcis.1993.1200View ArticleGoogle Scholar
- Feng X, Feng L, Jin M, Zhai J, Jiang L, Zhu D: J. Am. Chem. Soc.. 2004, 126: 62–63. COI number [1:CAS:528:DC%2BD3sXps1Gmt7s%3D] 10.1021/ja038636oView ArticleGoogle Scholar
- Pinzari F, Ascarellia P, Cappellia E, Matteia G, Giorgib R: Diam Relat Mater.. 2001, 10: 781. COI number [1:CAS:528:DC%2BD3MXjtFekt7o%3D] 10.1016/S0925-9635(00)00609-9View ArticleGoogle Scholar
- Vig JR: J. Vac. Sci. Technol. A.. 1985, 3: 1027. COI number [1:CAS:528:DyaL2MXksVejurc%3D]; Bibcode number [1985JVST....3.1027V] 10.1116/1.573115View ArticleGoogle Scholar
- Moon DW, Kurokawa A, Ichimura S, Lee HW, Jeon IC: J. Vac. Sci. Technol. A.. 1999, 17: 150. COI number [1:CAS:528:DyaK1MXit1Cktg%3D%3D]; Bibcode number [1999JVST...17..150M] 10.1116/1.581565View ArticleGoogle Scholar
- Apatiga LM, Velazques R, Castano VM: Surf. Sci.. 2003, 529: 158. COI number [1:CAS:528:DC%2BD3sXitVKlurk%3D]; Bibcode number [2003SurSc.529..158A] 10.1016/S0039-6028(03)00123-7View ArticleGoogle Scholar
- Hiller JJ: J. Appl. Phys.. 1947, 19: 226. Bibcode number [1948JAP....19..226H] 10.1063/1.1715049View ArticleGoogle Scholar
- Bakaev VA, Steele WA: J. Chem. Phys.. 1999, 111: 9803. COI number [1:CAS:528:DyaK1MXnsVaqtr4%3D]; Bibcode number [1999JChPh.111.9803B] 10.1063/1.480317View ArticleGoogle Scholar
- Leed EA, Sofo JO, Pantano CG: Phys. Rev. B.. 2005, 72: 155427. Bibcode number [2005PhRvB..72o5427L] 10.1103/PhysRevB.72.155427View ArticleGoogle Scholar
- Yoshiie T, Iwanaga H, Shibata N, Ichihara M, Takeuchi S: Philos. Mag.. 1979,A40(2):297. Bibcode number [1979PMagA..40..297Y]View ArticleGoogle Scholar